#------------------------------------------------------------------------------
#$Date: 2021-06-18 10:29:20 +0300 (Fri, 18 Jun 2021) $
#$Revision: 266558 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/35/1563562.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563562
loop_
_publ_author_name
'Wang, Yonggang'
'Li, R.K.'
_publ_section_title
;
 K2Fe2B2O7: A transparent nonlinear optical crystal with frustrated
 magnetism
;
_journal_issue                   6
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1221
_journal_page_last               1225
_journal_paper_doi               10.1016/j.jssc.2010.03.037
_journal_volume                  183
_journal_year                    2010
_chemical_formula_sum            'B2 Fe2 K2 O7'
_chemical_formula_weight         323.52
_chemical_melting_point          1014
_space_group_IT_number           150
_space_group_name_Hall           'P 3 2"'
_space_group_name_H-M_alt        'P 3 2 1'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   8.7475(12)
_cell_length_b                   8.7475(12)
_cell_length_c                   8.5124(17)
_cell_measurement_reflns_used    2093
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      27.4662
_cell_measurement_theta_min      3.6004
_cell_volume                     564.09(16)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      93(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0563
_diffrn_reflns_av_sigmaI/netI    0.0397
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            4534
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_diffrn_reflns_theta_min         3.60
_exptl_absorpt_coefficient_mu    4.957
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.7335
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'CrystalClear.Rigaku Corporation.(1997-2002)'
_exptl_crystal_colour            Yellow
_exptl_crystal_density_diffrn    2.857
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Chunk
_exptl_crystal_F_000             468
_exptl_crystal_size_max          0.167
_exptl_crystal_size_mid          0.167
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.495
_refine_diff_density_min         -0.672
_refine_diff_density_rms         0.130
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.03(3)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.984
_refine_ls_matrix_type           full
_refine_ls_number_parameters     61
_refine_ls_number_reflns         874
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.984
_refine_ls_R_factor_all          0.0282
_refine_ls_R_factor_gt           0.0240
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0207P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0523
_refine_ls_wR_factor_ref         0.0540
_reflns_number_gt                779
_reflns_number_total             874
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2010-183-1221.cif
_cod_data_source_block           br173
_cod_original_sg_symbol_H-M      P321
_cod_database_code               1563562
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.0000 0.0000 0.71048(8) 0.00454(17) Uani 1 3 d S . .
Fe2 Fe 0.6667 0.3333 0.80960(8) 0.00492(18) Uani 1 3 d S . .
Fe3 Fe 0.3333 0.6667 0.76756(8) 0.00508(17) Uani 1 3 d S . .
K1 K 0.68190(11) 0.0000 0.0000 0.0097(2) Uani 1 2 d S . .
K2 K 0.64708(11) 0.0000 0.5000 0.0097(2) Uani 1 2 d S . .
O1 O 0.0000 0.0000 0.5000 0.0132(11) Uani 1 6 d S . .
O2 O 0.3333 0.6667 0.9789(4) 0.0165(9) Uani 1 3 d S . .
O3 O 0.5630(3) 0.7391(3) 0.6991(3) 0.0103(5) Uani 1 1 d . . .
O4 O 0.8978(3) 0.4124(3) 0.7429(3) 0.0109(5) Uani 1 1 d . . .
O5 O 0.2283(3) 0.0669(3) 0.7810(3) 0.0101(5) Uani 1 1 d . . .
B1 B 0.0010(4) 0.3358(5) 0.7411(4) 0.0069(8) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Fe1 O5 108.66(7) . .
O1 Fe1 O5 108.66(7) . 3
O5 Fe1 O5 110.27(7) . 3
O1 Fe1 O5 108.66(7) . 2
O5 Fe1 O5 110.27(7) . 2
O5 Fe1 O5 110.27(7) 3 2
O1 Fe1 K2 59.870(14) . 2_545
O5 Fe1 K2 88.29(6) . 2_545
O5 Fe1 K2 64.26(7) 3 2_545
O5 Fe1 K2 161.10(7) 2 2_545
O1 Fe1 K2 59.870(14) . 1_455
O5 Fe1 K2 161.10(7) . 1_455
O5 Fe1 K2 88.29(6) 3 1_455
O5 Fe1 K2 64.26(7) 2 1_455
K2 Fe1 K2 97.011(18) 2_545 1_455
O1 Fe1 K2 59.870(14) . 3_665
O5 Fe1 K2 64.26(7) . 3_665
O5 Fe1 K2 161.10(7) 3 3_665
O5 Fe1 K2 88.29(6) 2 3_665
K2 Fe1 K2 97.011(18) 2_545 3_665
K2 Fe1 K2 97.011(18) 1_455 3_665
O1 Fe1 K1 131.531(15) . 3_666
O5 Fe1 K1 43.35(6) . 3_666
O5 Fe1 K1 117.88(7) 3 3_666
O5 Fe1 K1 67.85(7) 2 3_666
K2 Fe1 K1 131.036(7) 2_545 3_666
K2 Fe1 K1 131.036(7) 1_455 3_666
K2 Fe1 K1 71.661(18) 3_665 3_666
O1 Fe1 K1 131.531(14) . 1_456
O5 Fe1 K1 117.88(7) . 1_456
O5 Fe1 K1 67.85(7) 3 1_456
O5 Fe1 K1 43.35(6) 2 1_456
K2 Fe1 K1 131.036(7) 2_545 1_456
K2 Fe1 K1 71.661(18) 1_455 1_456
K2 Fe1 K1 131.036(7) 3_665 1_456
K1 Fe1 K1 80.83(2) 3_666 1_456
O1 Fe1 K1 131.531(14) . 2_546
O5 Fe1 K1 67.85(7) . 2_546
O5 Fe1 K1 43.35(6) 3 2_546
O5 Fe1 K1 117.88(7) 2 2_546
K2 Fe1 K1 71.661(18) 2_545 2_546
K2 Fe1 K1 131.036(7) 1_455 2_546
K2 Fe1 K1 131.036(7) 3_665 2_546
K1 Fe1 K1 80.83(2) 3_666 2_546
K1 Fe1 K1 80.83(2) 1_456 2_546
O2 Fe2 O4 107.69(7) 4_557 2_655
O2 Fe2 O4 107.69(7) 4_557 .
O4 Fe2 O4 111.19(7) 2_655 .
O2 Fe2 O4 107.69(7) 4_557 3_665
O4 Fe2 O4 111.19(7) 2_655 3_665
O4 Fe2 O4 111.19(7) . 3_665
O2 Fe2 K1 61.496(13) 4_557 2_656
O4 Fe2 K1 87.89(6) 2_655 2_656
O4 Fe2 K1 61.85(7) . 2_656
O4 Fe2 K1 160.68(7) 3_665 2_656
O2 Fe2 K1 61.498(13) 4_557 1_556
O4 Fe2 K1 160.68(7) 2_655 1_556
O4 Fe2 K1 87.89(6) . 1_556
O4 Fe2 K1 61.85(7) 3_665 1_556
K1 Fe2 K1 99.114(16) 2_656 1_556
O2 Fe2 K1 61.495(13) 4_557 3_666
O4 Fe2 K1 61.85(7) 2_655 3_666
O4 Fe2 K1 160.68(7) . 3_666
O4 Fe2 K1 87.89(6) 3_665 3_666
K1 Fe2 K1 99.114(16) 2_656 3_666
K1 Fe2 K1 99.114(16) 1_556 3_666
O2 Fe2 K2 132.921(11) 4_557 .
O4 Fe2 K2 115.90(7) 2_655 .
O4 Fe2 K2 72.79(7) . .
O4 Fe2 K2 40.38(7) 3_665 .
K1 Fe2 K2 134.114(17) 2_656 .
K1 Fe2 K2 71.585(14) 1_556 .
K1 Fe2 K2 126.49(2) 3_666 .
O2 Fe2 K2 132.920(11) 4_557 2_655
O4 Fe2 K2 72.78(7) 2_655 2_655
O4 Fe2 K2 40.38(7) . 2_655
O4 Fe2 K2 115.90(7) 3_665 2_655
K1 Fe2 K2 71.585(14) 2_656 2_655
K1 Fe2 K2 126.49(2) 1_556 2_655
K1 Fe2 K2 134.114(17) 3_666 2_655
K2 Fe2 K2 78.721(17) . 2_655
O2 Fe2 K2 132.919(11) 4_557 3_665
O4 Fe2 K2 40.38(7) 2_655 3_665
O4 Fe2 K2 115.90(7) . 3_665
O4 Fe2 K2 72.79(7) 3_665 3_665
K1 Fe2 K2 126.49(2) 2_656 3_665
K1 Fe2 K2 134.114(17) 1_556 3_665
K1 Fe2 K2 71.585(14) 3_666 3_665
K2 Fe2 K2 78.720(17) . 3_665
K2 Fe2 K2 78.721(17) 2_655 3_665
O2 Fe3 O3 108.15(7) . 2_665
O2 Fe3 O3 108.15(7) . 3_565
O3 Fe3 O3 110.76(7) 2_665 3_565
O2 Fe3 O3 108.14(7) . .
O3 Fe3 O3 110.76(7) 2_665 .
O3 Fe3 O3 110.76(7) 3_565 .
O2 Fe3 K1 56.459(12) . 1_566
O3 Fe3 K1 92.12(6) 2_665 1_566
O3 Fe3 K1 156.27(7) 3_565 1_566
O3 Fe3 K1 64.13(7) . 1_566
O2 Fe3 K1 56.459(12) . 2_556
O3 Fe3 K1 64.13(7) 2_665 2_556
O3 Fe3 K1 92.12(6) 3_565 2_556
O3 Fe3 K1 156.27(7) . 2_556
K1 Fe3 K1 92.410(16) 1_566 2_556
O2 Fe3 K1 56.459(12) . 3_666
O3 Fe3 K1 156.27(7) 2_665 3_666
O3 Fe3 K1 64.13(7) 3_565 3_666
O3 Fe3 K1 92.12(6) . 3_666
K1 Fe3 K1 92.410(16) 1_566 3_666
K1 Fe3 K1 92.410(16) 2_556 3_666
O2 Fe3 K2 128.787(11) . 2
O3 Fe3 K2 44.07(6) 2_665 2
O3 Fe3 K2 67.22(7) 3_565 2
O3 Fe3 K2 121.37(8) . 2
K1 Fe3 K2 136.119(19) 1_566 2
K1 Fe3 K2 72.490(15) 2_556 2
K1 Fe3 K2 128.20(2) 3_666 2
O2 Fe3 K2 128.787(12) . 1_565
O3 Fe3 K2 67.22(7) 2_665 1_565
O3 Fe3 K2 121.37(8) 3_565 1_565
O3 Fe3 K2 44.07(6) . 1_565
K1 Fe3 K2 72.490(15) 1_566 1_565
K1 Fe3 K2 128.204(19) 2_556 1_565
K1 Fe3 K2 136.119(19) 3_666 1_565
K2 Fe3 K2 84.916(17) 2 1_565
O2 Fe3 K2 128.787(12) . 3_665
O3 Fe3 K2 121.37(8) 2_665 3_665
O3 Fe3 K2 44.07(6) 3_565 3_665
O3 Fe3 K2 67.22(7) . 3_665
K1 Fe3 K2 128.204(19) 1_566 3_665
K1 Fe3 K2 136.119(19) 2_556 3_665
K1 Fe3 K2 72.490(15) 3_666 3_665
K2 Fe3 K2 84.916(17) 2 3_665
K2 Fe3 K2 84.916(17) 1_565 3_665
O5 K1 O5 112.42(10) 6_656 2_654
O5 K1 O2 87.29(6) 6_656 1_544
O5 K1 O2 129.73(7) 2_654 1_544
O5 K1 O2 129.73(7) 6_656 4_556
O5 K1 O2 87.29(6) 2_654 4_556
O2 K1 O2 115.70(3) 1_544 4_556
O5 K1 O4 167.59(6) 6_656 3_664
O5 K1 O4 74.34(7) 2_654 3_664
O2 K1 O4 80.54(6) 1_544 3_664
O2 K1 O4 59.22(7) 4_556 3_664
O5 K1 O4 74.34(7) 6_656 4_546
O5 K1 O4 167.59(6) 2_654 4_546
O2 K1 O4 59.22(7) 1_544 4_546
O2 K1 O4 80.53(6) 4_556 4_546
O4 K1 O4 101.10(8) 3_664 4_546
O5 K1 O3 73.20(6) 6_656 5_666
O5 K1 O3 104.73(6) 2_654 5_666
O2 K1 O3 125.43(7) 1_544 5_666
O2 K1 O3 56.87(6) 4_556 5_666
O4 K1 O3 116.03(6) 3_664 5_666
O4 K1 O3 66.48(5) 4_546 5_666
O5 K1 O3 104.73(6) 6_656 1_544
O5 K1 O3 73.20(6) 2_654 1_544
O2 K1 O3 56.87(6) 1_544 1_544
O2 K1 O3 125.43(7) 4_556 1_544
O4 K1 O3 66.48(5) 3_664 1_544
O4 K1 O3 116.03(6) 4_546 1_544
O3 K1 O3 176.42(8) 5_666 1_544
O5 K1 Fe2 65.80(5) 6_656 4_546
O5 K1 Fe2 158.60(4) 2_654 4_546
O2 K1 Fe2 31.95(6) 1_544 4_546
O2 K1 Fe2 110.48(4) 4_556 4_546
O4 K1 Fe2 103.95(5) 3_664 4_546
O4 K1 Fe2 33.23(4) 4_546 4_546
O3 K1 Fe2 95.22(4) 5_666 4_546
O3 K1 Fe2 86.46(4) 1_544 4_546
O5 K1 Fe2 158.60(4) 6_656 1_554
O5 K1 Fe2 65.80(5) 2_654 1_554
O2 K1 Fe2 110.48(4) 1_544 1_554
O2 K1 Fe2 31.95(6) 4_556 1_554
O4 K1 Fe2 33.23(4) 3_664 1_554
O4 K1 Fe2 103.95(5) 4_546 1_554
O3 K1 Fe2 86.46(4) 5_666 1_554
O3 K1 Fe2 95.22(4) 1_544 1_554
Fe2 K1 Fe2 124.13(3) 4_546 1_554
O5 K1 Fe3 108.04(4) 6_656 1_544
O5 K1 Fe3 100.64(5) 2_654 1_544
O2 K1 Fe3 30.10(6) 1_544 1_544
O2 K1 Fe3 113.10(4) 4_556 1_544
O4 K1 Fe3 59.80(4) 3_664 1_544
O4 K1 Fe3 86.47(4) 4_546 1_544
O3 K1 Fe3 151.85(5) 5_666 1_544
O3 K1 Fe3 31.36(4) 1_544 1_544
Fe2 K1 Fe3 62.05(2) 4_546 1_544
Fe2 K1 Fe3 93.01(2) 1_554 1_544
O5 K1 Fe3 100.64(5) 6_656 4_556
O5 K1 Fe3 108.04(4) 2_654 4_556
O2 K1 Fe3 113.10(4) 1_544 4_556
O2 K1 Fe3 30.10(6) 4_556 4_556
O4 K1 Fe3 86.47(4) 3_664 4_556
O4 K1 Fe3 59.80(4) 4_546 4_556
O3 K1 Fe3 31.36(4) 5_666 4_556
O3 K1 Fe3 151.84(5) 1_544 4_556
Fe2 K1 Fe3 93.01(2) 4_546 4_556
Fe2 K1 Fe3 62.04(2) 1_554 4_556
Fe3 K1 Fe3 127.24(3) 1_544 4_556
O3 K2 O3 162.29(10) 5_666 1_545
O3 K2 O4 111.41(7) 5_666 3_665
O3 K2 O4 79.41(7) 1_545 3_665
O3 K2 O4 79.41(7) 5_666 4_546
O3 K2 O4 111.41(7) 1_545 4_546
O4 K2 O4 107.94(10) 3_665 4_546
O3 K2 O1 81.14(5) 5_666 1_655
O3 K2 O1 81.14(5) 1_545 1_655
O4 K2 O1 126.03(5) 3_665 1_655
O4 K2 O1 126.03(5) 4_546 1_655
O3 K2 O5 96.13(7) 5_666 2_655
O3 K2 O5 73.87(6) 1_545 2_655
O4 K2 O5 70.06(6) 3_665 2_655
O4 K2 O5 174.18(6) 4_546 2_655
O1 K2 O5 56.23(4) 1_655 2_655
O3 K2 O5 73.87(6) 5_666 6_656
O3 K2 O5 96.13(7) 1_545 6_656
O4 K2 O5 174.18(6) 3_665 6_656
O4 K2 O5 70.07(6) 4_546 6_656
O1 K2 O5 56.23(4) 1_655 6_656
O5 K2 O5 112.46(8) 2_655 6_656
O3 K2 O3 60.06(8) 5_666 6_656
O3 K2 O3 137.42(4) 1_545 6_656
O4 K2 O3 79.29(6) 3_665 6_656
O4 K2 O3 43.88(6) 4_546 6_656
O1 K2 O3 140.41(4) 1_655 6_656
O5 K2 O3 130.53(5) 2_655 6_656
O5 K2 O3 101.94(5) 6_656 6_656
O3 K2 O3 137.42(4) 5_666 2_655
O3 K2 O3 60.06(8) 1_545 2_655
O4 K2 O3 43.88(6) 3_665 2_655
O4 K2 O3 79.29(6) 4_546 2_655
O1 K2 O3 140.41(4) 1_655 2_655
O5 K2 O3 101.94(5) 2_655 2_655
O5 K2 O3 130.53(5) 6_656 2_655
O3 K2 O3 79.18(7) 6_656 2_655
O3 K2 B1 74.61(8) 5_666 4_556
O3 K2 B1 120.76(8) 1_545 4_556
O4 K2 B1 89.13(8) 3_665 4_556
O4 K2 B1 22.37(7) 4_546 4_556
O1 K2 B1 143.03(6) 1_655 4_556
O5 K2 B1 152.67(7) 2_655 4_556
O5 K2 B1 89.99(7) 6_656 4_556
O3 K2 B1 23.40(6) 6_656 4_556
O3 K2 B1 71.72(7) 2_655 4_556
O3 K2 B1 120.76(7) 5_666 3
O3 K2 B1 74.61(8) 1_545 3
O4 K2 B1 22.37(7) 3_665 3
O4 K2 B1 89.13(8) 4_546 3
O1 K2 B1 143.03(6) 1_655 3
O5 K2 B1 89.99(7) 2_655 3
O5 K2 B1 152.67(7) 6_656 3
O3 K2 B1 71.72(7) 6_656 3
O3 K2 B1 23.40(6) 2_655 3
B1 K2 B1 73.93(12) 4_556 3
O3 K2 Fe1 100.93(5) 5_666 1_655
O3 K2 Fe1 62.87(5) 1_545 1_655
O4 K2 Fe1 97.39(5) 3_665 1_655
O4 K2 Fe1 152.74(5) 4_546 1_655
O1 K2 Fe1 30.129(14) 1_655 1_655
O5 K2 Fe1 31.54(4) 2_655 1_655
O5 K2 Fe1 83.73(4) 6_656 1_655
O3 K2 Fe1 156.61(3) 6_656 1_655
O3 K2 Fe1 114.53(4) 2_655 1_655
B1 K2 Fe1 173.16(6) 4_556 1_655
B1 K2 Fe1 112.91(6) 3 1_655
Fe1 O1 Fe1 180.0 4_556 .
Fe1 O1 K2 90.0 4_556 3_665
Fe1 O1 K2 90.0 . 3_665
Fe1 O1 K2 90.0 4_556 1_455
Fe1 O1 K2 90.0 . 1_455
K2 O1 K2 120.0 3_665 1_455
Fe1 O1 K2 90.0 4_556 2_545
Fe1 O1 K2 90.0 . 2_545
K2 O1 K2 120.0 3_665 2_545
K2 O1 K2 120.0 1_455 2_545
Fe3 O2 Fe2 180.0 . 4_557
Fe3 O2 K1 93.44(6) . 2_556
Fe2 O2 K1 86.56(6) 4_557 2_556
Fe3 O2 K1 93.44(6) . 1_566
Fe2 O2 K1 86.56(6) 4_557 1_566
K1 O2 K1 119.643(12) 2_556 1_566
Fe3 O2 K1 93.44(6) . 3_666
Fe2 O2 K1 86.56(6) 4_557 3_666
K1 O2 K1 119.643(12) 2_556 3_666
K1 O2 K1 119.643(12) 1_566 3_666
B1 O3 Fe3 126.3(2) 2_665 .
B1 O3 K2 127.33(19) 2_665 1_565
Fe3 O3 K2 106.32(9) . 1_565
B1 O3 K1 94.00(18) 2_665 1_566
Fe3 O3 K1 84.51(8) . 1_566
K2 O3 K1 92.65(6) 1_565 1_566
B1 O3 K2 79.49(18) 2_665 3_665
Fe3 O3 K2 82.12(7) . 3_665
K2 O3 K2 108.64(7) 1_565 3_665
K1 O3 K2 157.33(7) 1_566 3_665
B1 O4 Fe2 132.8(2) 1_655 .
B1 O4 K2 108.19(19) 1_655 2_655
Fe2 O4 K2 113.29(9) . 2_655
B1 O4 K1 112.46(19) 1_655 2_656
Fe2 O4 K1 84.92(8) . 2_656
K2 O4 K1 96.01(6) 2_655 2_656
B1 O5 Fe1 129.2(2) 3 .
B1 O5 K1 122.78(19) 3 3_666
Fe1 O5 K1 107.94(9) . 3_666
B1 O5 K2 96.46(19) 3 3_665
Fe1 O5 K2 84.20(8) . 3_665
K1 O5 K2 91.88(6) 3_666 3_665
O4 B1 O5 121.1(3) 1_455 2
O4 B1 O3 118.8(3) 1_455 3_565
O5 B1 O3 120.1(3) 2 3_565
O4 B1 K2 49.44(15) 1_455 2
O5 B1 K2 149.5(2) 2 2
O3 B1 K2 77.10(17) 3_565 2
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Fe1 O1 1.7917(8) .
Fe1 O5 1.877(2) .
Fe1 O5 1.877(2) 3
Fe1 O5 1.877(2) 2
Fe2 O2 1.800(3) 4_557
Fe2 O4 1.868(2) 2_655
Fe2 O4 1.868(2) .
Fe2 O4 1.868(2) 3_665
Fe3 O2 1.799(3) .
Fe3 O3 1.872(2) 2_665
Fe3 O3 1.872(2) 3_565
Fe3 O3 1.872(2) .
K1 O5 2.682(2) 6_656
K1 O5 2.682(2) 2_654
K1 O2 2.9901(7) 1_544
K1 O2 2.9901(7) 4_556
K1 O4 3.006(2) 3_664
K1 O4 3.006(2) 4_546
K1 O3 3.237(2) 5_666
K1 O3 3.237(2) 1_544
K2 O3 2.635(2) 5_666
K2 O3 2.635(2) 1_545
K2 O4 2.730(2) 3_665
K2 O4 2.730(2) 4_546
K2 O1 3.0872(10) 1_655
K2 O5 3.232(2) 2_655
K2 O5 3.232(2) 6_656
K2 O3 3.384(2) 6_656
K2 O3 3.384(2) 2_655
O1 Fe1 1.7917(8) 4_556
O1 K2 3.0872(10) 3_665
O1 K2 3.0872(10) 1_455
O1 K2 3.0872(10) 2_545
O2 Fe2 1.800(3) 4_557
O2 K1 2.9901(7) 2_556
O2 K1 2.9901(7) 1_566
O2 K1 2.9901(7) 3_666
O3 B1 1.379(4) 2_665
O3 K2 2.635(2) 1_565
O3 K1 3.237(2) 1_566
O3 K2 3.384(2) 3_665
O4 B1 1.367(4) 1_655
O4 K2 2.730(2) 2_655
O4 K1 3.006(2) 2_656
O5 B1 1.375(4) 3
O5 K1 2.682(2) 3_666
O5 K2 3.232(2) 3_665
B1 O4 1.367(4) 1_455
B1 O5 1.375(4) 2
B1 O3 1.379(4) 3_565
